PPT02-notes_probs

# PPT02-notes_probs - ME4 Polymer Processing Technology 2...

This preview shows pages 1–3. Sign up to view the full content.

2 Melt rheology and rheometry Two main groups of material property data are needed to analyse and simulate Fow in the injection moulding process: 1 Properties of resistance to Fow under stress ( rheology ): expressed by shear stress vs . shear strain rate data; 2 Properties of static compressibility and thermal expansion: expressed using PVT data. These notes deal with the ±rst group: rheological properties and their measurement ( rheometry ). Rheometric methods have to be simple and analysable, so they provide a clear introduction to the analysis of melt Fow in injection moulding and a warning about possible problems. Learning outcomes After completing this section you should be able to… 1 Demonstrate an understanding of the theoretical basis and practical application of a Capillary Rheometer and a Cone and Plate rheometer. 2 Manipulate power-law, Cross, Cross-Arrhenius and Cross-WL² constitutive equations for polymer melts, and use them to represent data. 3 Assess whether Bagley or Rabinowitsch corrections are needed in calculations for polymer melt Fow in channels (e.g. rheometer capillaries, mould runners and gates), and apply them if necessary. 4 Demonstrate understanding and make appropriate use of the following terminology: apparent viscosity, Bagley correction, consistency, Cross model, degradation, die, extensional Fow, extensional viscosity, Fow curve, melt, melt slip, M²I, newtonian viscosity, power-law Fow, pseudoplasticity, Rabinowitsch correction, reference viscosity, reference shear rate, jetting, rheometer (capillary, cone-plate), shear rate (= shear strain rate), temperature coe³cient of viscosity, viscometer = rheometer, zero-shear viscosity. 2.1 Revision SPAP introduced: 1 The MFI test : a widely-used industrial test which provides a single-point ‘index’ of melt viscosity. ME4 Polymer Processing Technology PSL 19 October 2009

This preview has intentionally blurred sections. Sign up to view the full version.

View Full Document
Barrel of diameter 9.57 mm Capillary die length = 8.0 mm diameter = 2.09 mm Melt Fow index (M±I) = weight (in grams) extruded in 10 min Barrel heaters Melt at speci²ed temperature Total mass M 2 The cone-and-plate viscometer : an easily understood but very limited method for measuring melt viscosity at a controlled range of shear rates. 3 The capillary rheometer : a rheometric method which is much more powerful, but more di³cult to analyse. 4 Flow curves , representing viscosity data and showing that melts are very viscous, non-Newtonian (pseudoplastic) and temperature sensitive. 2.2 Melt ﬂow processes During injection moulding, a polymer melt meets a very wide range of processing variables (shear strain rate, temperature, pressure etc.). ±inding methods to measure and represent melt rheology across this range is a serious challenge. There are two basic classes of high-viscosity Fow. Most real Fow processes are mixed, but one form usually dominates.
This is the end of the preview. Sign up to access the rest of the document.

## This note was uploaded on 04/07/2010 for the course MECH ENG 207 taught by Professor Levers during the Fall '10 term at Imperial College.

### Page1 / 16

PPT02-notes_probs - ME4 Polymer Processing Technology 2...

This preview shows document pages 1 - 3. Sign up to view the full document.

View Full Document
Ask a homework question - tutors are online